ASTM-A967 › Standard Specification for Chemical Passivation Treatments for Stainless Steel Parts
Show Complete Document History
The following bibliographic material is provided to assist you with your purchasing decision:
This specification covers several different types of chemical passivation treatments for stainless steel parts. The treatments are the following: immersion treatment using nitric acid solutions, immersion treatment using citric acid solution, and electrochemical treatment. Immediately after the removal from the passivating solution, the parts shall be thoroughly rinsed, using stagnant, countercurrent, or spray washes, singly or in combination, with or without a separate chemical treatment for neutralization of the passivation media. The chemical reactions of the passivating media on the surface of the stainless steel shall be stopped by rinsing of the stainless steel part, with or without a separate neutralization treatment. A chemical treatment shall be applied which will accelerate the formation of the passive film on a chemically clean stainless steel surface. The passivated parts shall exhibit a chemically clean surface and shall, on visual inspection, show no etching, pitting, or frosting. The following tests shall be performed on each lot of stainless steel parts: water immersion test, high humidity test, salt spray test, copper sulfate test, and potassium ferricyanide-nitric acid test. A free iron test shall be used for the detection of free iron on the surface of stainless steel.
Changes from the previous issue
A redline edition is available for this document, with all changes visible. Ask Document Center Inc. for more information.
1.1 This specification covers several different types of chemical passivation treatments for stainless steel parts. It includes recommendations and precautions for descaling, cleaning, and passivation of stainless steel parts. It includes several alternative tests, with acceptance criteria, for confirmation of effectiveness of such treatments for stainless steel parts.
1.2 Practices for the mechanical and chemical treatments of stainless steel surfaces are discussed more thoroughly in Practice .
1.3 Several alternative chemical treatments are defined for passivation of stainless steel parts. give some nonmandatory information and provides some general guidelines regarding the selection of passivation treatments appropriate to particular grades of stainless steel. This specification makes no recommendations regarding the suitability of any grade, treatment, or acceptance criteria for any particular application or class of applications.
1.4 The tests in this specification are intended to confirm the effectiveness of passivation, particularly with regard to the removal of free iron and other exogenous matter. These tests include the following practices:
1.4.1 Practice A—Water Immersion Test,
1.4.2 Practice B—High Humidity Test,
1.4.3 Practice C—Salt Spray Test,
1.4.4 Practice D—Copper Sulfate Test,
1.4.5 Practice E—Potassium Ferricyanide-Nitric Acid Test, and
1.4.6 Practice F—Damp Cloth Test, and
1.4.7 Practice G—Boiling Water Immersion Test.
Note 1: Free iron denotes iron present on the surface of the parts, including but not limited to iron contamination, iron-tool marks, residual-iron salts from pickling solutions, iron dust, atmospheric exposure, iron deposits in welds, embedded iron, and iron oxide.
1.5 The values stated in either SI units or inch-pound units are to be regarded separately as standard. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in non-conformance with the standard.
1.6 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
1.7 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
Changes to the new 2013 Edition of A967/A967M can be found in the following areas: Section 1.5 (changed to combined Metric/US units), Revised Section 4.1 and added Section 4.3, Added Notes 2 and 3 to Sections 6 and 7, Revised Section 13.3, Combined Sections 14 through 19 into a new Section 14, Revised Section 22.1 (Now numbered 17.1) and added Section 17.2, and Added Sections X1.3.2-X1.3.4 and X1.12 to the Appendix.
This practice references QQ-P-35 (later renumbered AMS-QQ-P-35 and then withdrawn in favor of AMS-2700), another major passivation document. The ASTM A967/A967-13 replaces ASTM A967/A967M-05 which is now obsolete.
cleaning of stainless steel; passivation; passivation tests; tests for cleanliness of stainless steels;; ICS Number Code 77.140.20 (Steels of high quality)
To find similar documents by ASTM Volume:
To find similar documents by classification:
This document comes with our free Notification Service, good for the life of the document.
This document is available in either Paper or PDF format.
Customers who bought this document also bought:
Standard Specification for Chromium and Chromium-Nickel Stainless Steel Plate, Sheet, and Strip for Pressure Vessels and for General Applications
Quality management systems - Requirements
Sampling Procedures and Tables for Inspection by Attributes - Paper Format - Reaffirmed in 2018
July 15, 2017